Synchrotron X-ray analysis of the electron density in CoF~2~ and ZnF~2~
O'Toole, Nicholas J.; Streltsov, Victor A.; Acta Crystallographica Section B 57 (2001) 128–135; doi:10.1107/S0108768100017353

data_2103614
_publ_section_title
;
 Synchrotron X-ray analysis of the electron density in CoF~2~ and
 ZnF~2~
;
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              128
_journal_page_last               135
_journal_paper_doi               10.1107/S0108768100017353
_journal_volume                  57
_journal_year                    2001
_chemical_formula_sum            'Co F2'
_chemical_formula_weight         12.1161
_space_group_IT_number           136
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_audit_creation_method           from_xtal_archive_file_using_CIFIO
_cell_angle_alpha                90.000(8)
_cell_angle_beta                 90.000(8)
_cell_angle_gamma                90.000(8)
_cell_formula_units_Z            16
_cell_length_a                   4.6956(5)
_cell_length_b                   4.6956(5)
_cell_length_c                   3.1793(3)
_cell_measurement_reflns_used    6
_cell_measurement_temperature    293
_cell_measurement_theta_max      52.43
_cell_measurement_theta_min      45.69
_cell_volume                     70.099(12)
_computing_data_reduction        'xtal DIFDAT ADDREF SORTRF ABSORB'
_computing_molecular_graphics    xtal
_computing_publication_material  'xtal CIFIO'
_computing_structure_refinement  'xtal CRYLSQ'
_computing_structure_solution    xtal
_diffrn_ambient_temperature      293
_diffrn_measurement_device       'BL14A Four circle'
_diffrn_measurement_method       \w-2\q
_diffrn_radiation_monochromator  si(111)
_diffrn_radiation_source         'Photon Factory BL14A'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     .84
_diffrn_reflns_av_R_equivalents  .039
_diffrn_reflns_av_sigmaI/netI    .021
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            2883
_diffrn_reflns_theta_max         67.4
_diffrn_reflns_theta_min         7.27
_diffrn_standards_decay_%        3
_diffrn_standards_interval_count 94
_diffrn_standards_number         6
_exptl_absorpt_coefficient_mu    18.22
_exptl_absorpt_correction_T_max  .864
_exptl_absorpt_correction_T_min  .801
_exptl_absorpt_correction_type   analytical
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    4.592
_exptl_crystal_description       rectangular
_exptl_crystal_F_000             90
_refine_diff_density_max         1.166
_refine_diff_density_min         -1.067
_refine_ls_extinction_coef       91E2(8)
_refine_ls_extinction_method     Zachariasen
_refine_ls_goodness_of_fit_all   2.416
_refine_ls_goodness_of_fit_obs   2.416
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     9
_refine_ls_number_reflns         235
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          .019
_refine_ls_R_factor_obs          .019
_refine_ls_shift/esd_max         .00005
_refine_ls_shift/esd_mean        .00001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/\s^2^(F)
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         .015
_refine_ls_wR_factor_obs         .015
_reflns_number_observed          2502
_reflns_number_total             2883
_reflns_observed_criterion       'I > 2\s(I)'
_cod_data_source_file            os0063.cif
_cod_data_source_block           cof2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'w=1/\s^2^(F)' was changed to
'calc'. New tag '_refine_ls_weighting_details' was created. The value
of the new tag was set to 'w=1/\s^2^(F)'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        70.099(16)
_cod_database_code               2103614
_cod_database_fobs_code          2103614